We have shown that the transverse magnetoresistivity inside the hidden-order phase of URu2Si2 strongly depends on the sample quality. In fact, the orbital effect is en-hanced when the mobility, proportional to the relaxation time (see Sect. 2.4), of the charge carriers is higher. The relaxation timeτ increases with the purity of the sam-ples and decreases with the temperature. An almost perfect compensation of elec-trons and holes in URu2Si2is shown by the monotonously-increasing transverse mag-netoresistivity in fields µ0H∥aup to 80 T (see Fig. 7.2). Assuming that the elec-tronic properties can be described by a unique relaxation time and an average mobil-ity for all conduction bands, the magnetoresistivmobil-ity ∆ρx,x=ρx,x(H)−ρnx,x(H = 0) of a compensated metal with spherical Fermi surfaces is given by (see Sect. 2.4):
ρnx,x(H= 0) = (ωcτ)2 =µ2(µ0H)2, (7.1) whereρnx,x is the zero-field resistivity estimated for the normal non-superconducting state (virtual normal state at temperatures below TSC, see Sect. 3.5).
7.4 Analysis of the magnetoresistivity T = 100 mK and (b)T = 1.4 K. The scattered lines representH2-dependencies.
∆ρx,x/ρnx,x(H = 0) of samples (c) #1 and (d) #2 versus (µ0H)2 in µ0H∥ c up to 20 T, at temperatures from 100 mK to 6 K.
Kasahara et al. [Kasahara 2007] have found, for a high-quality sample [RRR∗ = ρx,x(300 K)/ρx,x(T → 0) = 670], a nearly perfect ∝ H2-dependence of ∆ρx,x in magnetic fieldsµ0H∥c up to 10 T and Levallois et al. [Levallois 2009] have found for a sample of lower quality [RRR =ρx,x(300K)/ρx,x(2K) = 40], a field-dependence of ∆ρx,x close to ∝ H2 in fields H ∥ c up to µ0H = 20 T. The resistivity of our high-quality URu2Si2 sample #2 increases by more than two orders of magnitude in magnetic fields applied along a and c, as shown in Figures 7.2(a) and 7.3(a), respectively. This exceptionally-strong transverse magnetoresistivity is due to a very low carrier density [Levallois 2009] combined with the high sample-qualities [Kasahara 2007, Matsuda 2011].
Figure 7.6 shows plots of the magnetoresistivity of samples #1 and #2 versus H2 for µ0H ∥ c up to 20 T at different temperatures from 100 mK to 6 K. The plots show aH2-dependence ofρx,x in low fields between∼3 and 13 T in agreement with
7 Orbital Magnetoresistivity Levallois et al. (RRR = 40) [Levallois 2009]. The mobilities were extracted from by the slope ofρ(H) versus (µ0H)2 in H∥c[see Fig. 7.6]. The dashed lines are guides to the eyes. Mobility µ of samples #1 and #2 versus (c) T and (d) 1/ρnx,x(H = 0). The dashed lines are guides to the eyes.
the results of Kasahara et al. [Kasahara 2007] and Levallois et al. [Levallois 2009].
On the other hand, the behavior of the magnetoresistivity clearly deviates from the H2-dependence at higher fields. As the maximum in the resistivity at ∼30 T [see Fig. 7.3(a)], the slope of the low-field H2-dependence is enhanced with the sample quality. I extracted a mobility µ averaged over all bands by fitting ρxx versus H2, in the regime between 3 and 13 T, using Equation (7.1). I note here, that for temperatures below TSC = 1.5 K, the zero-field resistivity ρnx,x(H = 0) of the normal non-superconducting state was obtained by the extrapolation via a fit ρx,x(T) = ρ0 +AT1.5 to the resistivity between 1.5 and 8 K (see Sect. 3.5 and [Matsuda 2011]). I found similar RRR-dependencies of the resistivity maximum at Hρ,maxLT [see Fig. 7.7(a)] and of the mobility [see Fig. 7.7(b)], both being strongly enhanced with a higher sample quality. Figure 7.7(c) shows the mobility µ versus
7.4 Analysis of the magnetoresistivity the temperature T extracted for samples #1 (RRR = 90) and #2 (RRR = 225) inH∥c. The mobility is enhanced as the temperature decreases and a saturation occurs due to a finite relaxation time in the limit of zero temperature (non-perfect crystals). Figure 7.7(d) shows that the mobilitiesµof samples #1 and #2 increase approximately linearly with 1/ρnx,x(H= 0), which is compatible with the picture of an isotrope metal with a unique relaxation time τ, where τ ∝1/ρnx,x(H = 0) (see Sect. 2.4).
The Kohler’s rule [Kohler 1938] implies that all plots of ∆ρx,x(H)/ρnx,x(H = 0) versus [µ0H/ρnx,x(H = 0)]2 fall on a unique curve, which is independent of the sample quality and the temperature (see Sect. 2.4.4). Levalloiset al. [Levallois 2009]
have shown that the Kohler plots from the resistivity of their sample (RRR = 40) at temperatures between 1.5 and 17 K in fields µ0H ∥ c up to 20 T fall on a same [µ0H/ρnx,x(H = 0)]2-line. Figures 7.8(a) and (b) show the Kohler plots of the resistivities of our samples #1 and #2, respectively, in fieldsµ0H ∥ c up to 20 T, at temperatures from 100 mK to 6 K. For sample #1, the plots coincide almost up to 20 T and a H2-dependence is clearly observed. For sample #2, the plots coincide in a smaller field window (up to∼10 T) and deviate faster in higher fields from theH2-dependence than for sample #1. Figures 7.8(c) and (d) show the same plots forµ0H up to 40 T in a double-logarithmic scale. These plots emphasize that the magnetoresistivity behavior changes drastically at low fields in the proximity of Hc2 and at the field-induced crossoversH∗ and Hρ,maxLT . The deviation from the H2-dependence at low fields is due to the combination of the proximity ofHc2 and a parasitic off-set in the raw resistivity data. Figures 7.8(e) and (f) compare the Kohler plots of the resistivities of samples #1 and #2 and that from the sample studied by Levallois et al. [Levallois 2009] in a double-logarithmic scale, at T = 100 mK andT = 1.4 K, respectively. The plots of the different samples are close but do not coincide in the low-field regime.
To summarize, the low-field magnetoresistivity exhibits aH2-behavior, as predicted for a metal with a compensated spherical Fermi surface (cf. also [Pippard 1989, Kasahara 2007, Levallois 2009]). The extracted mobility depends on the sample quality and the temperature. On the other hand, the high-field magnetoresistiv-ity ∆ρ(H)/ρ(H = 0) deviates strongly from the H2-behavior, namely, when field-induced crossover-like anomalies in the magnetoresistivity occur atµ0H∗ ∼20−25 T and µ0Hρ,maxLT ∼ 30 T. In fact, URu2Si2 has a complex multi-band structure (see Sect. 9.1) and field-induced Fermi surface modifications have been observed in mag-netic fields far below the destruction of the hidden-order phase atµ0H1= 35 T (see Sect. 9.2). ForH∥a, I could not analyze the magnetoresistivity, as done forH∥c, because of a lack of reproducibility between the different sets of data (cf. Sect 3.9).
7 Orbital Magnetoresistivity
[Lev allois et al.]
sample double-logarithmic scale. The scattered lines representH2-dependencies.
7.4 Analysis of the magnetoresistivity For H∥a, the slope of the low-field magnetoresistivity is stronger and indicates a mobility higher than forH∥c [see also Chapt. 8, Fig. 8.4(b)]. Since the mobility is inversely proportional to the cyclotron effective mass (see Sect. 2.4), a higher mobility forH∥athan forH∥cis compatible with the anisotropy of the cyclotron effective masses extracted by Shubnikov-de Haas experiments [Aoki 2012].
8 Angle-Dependent Study of the High-Field Magnetoresistivity
URu2Si2 exhibits strongly anisotropic bulk properties due to the Ising-character of its magnetic properties. The magnetic easy axis is the c-axis of the body-centered tetragonal lattice. This results in strongly anisotropic re-sistivity [Palstra 1986, Ohkuni 1997] and magnetic susceptibility [Palstra 1985, Dawson 1989, Ramirez 1992]. The upper critical field Hc2 related to the destruc-tion of superconductivity is also strongly anisotropic [Kwok 1990, Brison 1994, Ohkuni 1997]. Magnetization [Sugiyama 1990] and magnetoresistivity [Jo 2007]
measurements have shown that the low-temperature critical fieldsH1, H2, and H3 follow a simple 1/cosθ-law, at least up toθ= 30◦, whereθis the angle between the magnetic field and the c-axis. Furthermore, Aoki et al. [Aoki 2012] observed that the crossover field H∗ in the magnetoresistivity also follows a 1/cosθ-law, at least up to θ= 30◦. In this chapter, I present magnetoresistivity experiments performed on the URu2Si2 monocrystalline samples #1 and #2 in a rotation probe, which per-mitted to measure the magnetoresistivity versus a magnetic field up to 60 T applied along different orientations of the crystal. The basic crystal planes (a,c) and (a,c) of the tetragonal structure have been investigated. These experiments extended the angle-dependence of the transition fields H1, H2, and H3 and the crossover fields H∗ and Hρ,maxLT up to θ= 60◦.
8.1 Angle dependence of Hc2
Figure 8.1(a) presents the transverse magnetoresistivity ρx,x of our sample #2 of URu2Si2versus the magnetic fieldHapplied parallel to the (a,c)-plane, for different angles θ between the magnetic field and the c-axis at T = 32 mK. The resistivity equals zero below the superconducting critical fieldHc2 and increases monotonically above Hc2. The critical field µ0Hc2 equals 3.1 T for θ = 5◦ and increases with θ, reaching 7.1 T for θ = 67◦. In the normal conducting state, ρx,x(H) exhibits an oscillatory modulation due to the Shubnikov-de Haas effect, which will be analyzed in Chapter 9. The θ-dependence ofHc2 obtained by our resistivity experiments on sample #2 is plotted in Figure 8.1(b). Hc2 exhibits a pronounced anisotropy in the
8 Angle-Dependent Study of the High-Field Magnetoresistivity
Figure 8.1: (a) Magnetoresistivityρx,x of URu2Si2sample #2 versus the magnetic fieldH for different anglesθbetweenHandcatT = 32 mK. (b) Angle-dependence of Hc2 forHin the plane (a,c) from our resistivity data of sample #2 and from resistivity data from [Ohkuni 1999]. ∗The solid lines represent fits to the data with the function (8.1).
(a,c)-plane. The angle dependence ofHc,2 obtained by Ohkuniet al. [Ohkuni 1999]
on another sample, also plotted in Fig. 8.1(b), is in good agreement with that from our data. The data of Ohkuni et al. [Ohkuni 1999] show that, at T = 30 mK, µ0Hc2 reaches ≃ 13 T for H ∥ a (θ = 90◦). The angle dependence of Hc,2 was first established by Brison et al. [Brison 1994] from specific heat measurements.
They proposed a theoretical model for the anisotropy of Hc2, based on the Pauli paramagnetic limit:
Hc2(θ) = Hc2(H∥c)
√cos2(θ) +ϵ2sin2(θ), (8.1) where ϵ = Hc2(H ∥ c)/Hc2(H ∥ a), and found that this model fits well to their data at T = 10 mK. The angle-dependencies of Hc,2 established by Ohkuni et al.
[Ohkuni 1999] and in this work are well described by this model, too [see Fig. 8.1(b)].